NaBaM<sup>III</sup>Q<sub>3</sub> (M<sup>III</sup> = Al, Ga; Q = S, Se): first quaternary chalcogenides with isolated edge-sharing (MQ<sub>6</sub>)<sup>6-</sup> dimers.
Abudurusuli, Ailijiang; Wu, Kui; Rouzhahong, Yilimiranmu; Yang, Zhihua; Pan, Shilie; Dalton transactions (Cambridge, England : 2003) 47 (2018) 16044–16047; doi:10.1039/c8dt04048f

data_7047866
_publ_section_title
;
 NaBaM<sup>III</sup>Q<sub>3</sub> (M<sup>III</sup> = Al, Ga; Q = S, Se):
 first quaternary chalcogenides with isolated edge-sharing
 (MQ<sub>6</sub>)<sup>6-</sup> dimers.
;
_journal_issue                   45
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              16044
_journal_page_last               16047
_journal_paper_doi               10.1039/c8dt04048f
_journal_volume                  47
_journal_year                    2018
_chemical_formula_sum            'Ba2 Ga2 Na2 Se6'
_chemical_formula_weight         933.87
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2018-07-18 deposited with the CCDC.
2018-10-10 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   20.461(13)
_cell_length_b                   9.177(6)
_cell_length_c                   7.177(4)
_cell_measurement_reflns_used    1274
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.08
_cell_measurement_theta_min      2.98
_cell_volume                     1347.6(14)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'Bruker SHELXTL'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0542
_diffrn_reflns_av_sigmaI/netI    0.0436
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            7885
_diffrn_reflns_theta_full        27.56
_diffrn_reflns_theta_max         27.56
_diffrn_reflns_theta_min         2.98
_exptl_absorpt_coefficient_mu    25.939
_exptl_absorpt_correction_T_max  0.9342
_exptl_absorpt_correction_T_min  0.7234
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.603
_exptl_crystal_description       block
_exptl_crystal_F_000             1600
_exptl_crystal_size_max          0.187
_exptl_crystal_size_mid          0.122
_exptl_crystal_size_min          0.087
_refine_diff_density_max         1.174
_refine_diff_density_min         -1.296
_refine_diff_density_rms         0.245
_refine_ls_extinction_coef       0.00047(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.026
_refine_ls_matrix_type           full
_refine_ls_number_parameters     68
_refine_ls_number_reflns         1652
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.026
_refine_ls_R_factor_all          0.0408
_refine_ls_R_factor_gt           0.0271
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0080P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0447
_refine_ls_wR_factor_ref         0.0487
_reflns_number_gt                1307
_reflns_number_total             1652
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c8dt04048f2.cif
_cod_data_source_block           22
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7047864--7047867.cif.

2023-11-21
Z value and formula fixed to values more according to usual
chemical conventions.                 miguel
;
_cod_original_formula_sum            'Ba0.73 Ga0.73 Na0.73 Se2.18'
_cod_original_formula_weight         339.59
_cod_original_formula_units_Z            11
_cod_original_sg_symbol_H-M      'Pnma '
_cod_database_code               7047866